ASTM e 1417
ASTM E1417 / E1417M – 11e1 Standard Practice for Liquid Penetrant Testing
ASTM E1417 / E1417M
Significance and Use ASTM e 1417 pdf
This practice establishes the basic parameters for controlling the application of the liquid penetrant method. This practice is written so it can be specified on the engineering drawing, specification, or contract. It is not a detailed how-to procedure to be used by the inspector and, therefore, must be supplemented by a detailed procedure that conforms to the requirements of this practice. Specification E165 contains information to help develop detailed requirements.
1.1 This practice establishes the minimum requirements for conducting liquid penetrant examination of nonporous metal, and nonmetal components.
Note 1—This practice replaces MIL-STD-6866.
1.2 The penetrant examination processes described in this practice are applicable to in-process, final, and maintenance (in-service) examinations. These processes are applicable for the detection of discontinuities, such as lack of fusion, corrosion, cracks, laps, cold shuts, and porosity, that are open or connected to the surface of the component under examination.
1.3 Caution must be exercised in the usage of elevated temperature with components manufactured from thermoplastic materials. Also, some cleaners, penetrants, and developers can have a deleterious effect on nonmetallic materials such as plastics. Prior to examination, tests should be conducted to ensure that none of the cleaning or examination materials are harmful to the components to be examined.
1.4 Units—The values stated in either SI units or inch-pound units are to be regarded separately as standard. The values stated in each system may not be exact equivalents; therefore, each system shall be used independently of the other. Combining values from the two systems may result in non-conformance with the standard.
1.5 All areas of this practice may be open to agreement between the cognizant engineering organization and the supplier, or specific direction from the cognizant engineering organization.
1.6 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
dye liquid penetrant examination; dye penetrant examination; fluorescent liquid penetrant examination; fluorescent penetrant examination; liquid penetrant examination; liquid penetrant examination; liquid penetrant testing; nondestructive; nondestructive evaluation; nondestructive examination; nondestructive examination; nondestructive testing; penetrant examination; penetrant examination; penetrant testing; Discontinuities; Dye penetrant inspection; Engineering applications; Fluorescent liquid penetrant testing; Hydrophilic emulsifiers; Karl Fischer reagent method; Lipophilic emulsification; Liquid penetration; Metals and metallic materials; Nondestructive evaluation (NDE); Nonmetallic materials; Nonporous materials; Penetrant inspection; Surface analysis–metals/alloy